The crystal structure described by Sr2ZrVO6 is (Cubic) Perovskite-derived structured and crystallizes in the monoclinic Pm space group. There are four inequivalent Sr sites. In the first Sr site, Sr(1) is bonded to one O(10), one O(13), one O(14), one O(17), one O(2), one O(20), one O(4), one O(5), one O(8), one O(9), and two equivalent O(1) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(1)O12 cuboctahedra, corners with two equivalent Sr(3)O12 cuboctahedra, corners with four equivalent Sr(2)O12 cuboctahedra, corners with four equivalent Sr(4)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(2)O6 octahedra,  a faceface with one Zr(4)O6 octahedra,  a faceface with one V(1)O6 octahedra,  a faceface with one V(3)O6 octahedra, faces with two equivalent Zr(1)O6 octahedra, and faces with two equivalent V(4)O6 octahedra. In the second Sr site, Sr(2) is bonded to one O(1), one O(10), one O(11), one O(14), one O(15), one O(17), one O(18), one O(3), one O(5), one O(6), and two equivalent O(2) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(2)O12 cuboctahedra, corners with two equivalent Sr(4)O12 cuboctahedra, corners with four equivalent Sr(1)O12 cuboctahedra, corners with four equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra,  a faceface with one Zr(1)O6 octahedra,  a faceface with one Zr(3)O6 octahedra,  a faceface with one V(2)O6 octahedra,  a faceface with one V(4)O6 octahedra, faces with two equivalent Zr(2)O6 octahedra, and faces with two equivalent V(1)O6 octahedra. In the third Sr site, Sr(3) is bonded to one O(11), one O(12), one O(15), one O(16), one O(18), one O(19), one O(2), one O(4), one O(6), one O(7), and two equivalent O(3) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(1)O12 cuboctahedra, corners with two equivalent Sr(3)O12 cuboctahedra, corners with four equivalent Sr(2)O12 cuboctahedra, corners with four equivalent Sr(4)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(2)O6 octahedra,  a faceface with one Zr(4)O6 octahedra,  a faceface with one V(1)O6 octahedra,  a faceface with one V(3)O6 octahedra, faces with two equivalent Zr(3)O6 octahedra, and faces with two equivalent V(2)O6 octahedra. In the fourth Sr site, Sr(4) is bonded to one O(1), one O(12), one O(13), one O(16), one O(19), one O(20), one O(3), one O(7), one O(8), one O(9), and two equivalent O(4) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(2)O12 cuboctahedra, corners with two equivalent Sr(4)O12 cuboctahedra, corners with four equivalent Sr(1)O12 cuboctahedra, corners with four equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(1)O6 octahedra,  a faceface with one Zr(3)O6 octahedra,  a faceface with one V(2)O6 octahedra,  a faceface with one V(4)O6 octahedra, faces with two equivalent Zr(4)O6 octahedra, and faces with two equivalent V(3)O6 octahedra. There are four inequivalent Zr sites. In the first Zr site, Zr(1) is bonded to one O(13), one O(17), one O(5), one O(9), and two equivalent O(1) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(3)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(1)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. In the second Zr site, Zr(2) is bonded to one O(10), one O(14), one O(18), one O(6), and two equivalent O(2) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(2)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-9°. In the third Zr site, Zr(3) is bonded to one O(11), one O(15), one O(19), one O(7), and two equivalent O(3) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(3)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(3)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-6°. In the fourth Zr site, Zr(4) is bonded to one O(12), one O(16), one O(20), one O(8), and two equivalent O(4) atoms to form ZrO6 octahedra that share corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(3)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(4)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-9°. There are four inequivalent V sites. In the first V site, V(1) is bonded to one O(11), one O(15), one O(17), one O(5), and two equivalent O(2) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(2)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-6°. In the second V site, V(2) is bonded to one O(12), one O(16), one O(18), one O(6), and two equivalent O(3) atoms to form VO6 octahedra that share corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(3)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-9°. In the third V site, V(3) is bonded to one O(13), one O(19), one O(7), one O(9), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(4)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. In the fourth V site, V(4) is bonded to one O(10), one O(14), one O(20), one O(8), and two equivalent O(1) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(1)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. There are twenty inequivalent O sites. In the first O site, O(1) is bonded in a distorted linear geometry to one Sr(2), one Sr(4), two equivalent Sr(1), one Zr(1), and one V(4) atom. In the second O site, O(2) is bonded in a distorted linear geometry to one Sr(1), one Sr(3), two equivalent Sr(2), one Zr(2), and one V(1) atom. In the third O site, O(3) is bonded in a distorted linear geometry to one Sr(2), one Sr(4), two equivalent Sr(3), one Zr(3), and one V(2) atom. In the fourth O site, O(4) is bonded in a distorted linear geometry to one Sr(1), one Sr(3), two equivalent Sr(4), one Zr(4), and one V(3) atom. In the fifth O site, O(5) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(1), and one V(1) atom. In the sixth O site, O(6) is bonded in a 2-coordinate geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(2), and one V(2) atom. In the seventh O site, O(7) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(3), and one V(3) atom. In the eighth O site, O(8) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(4), and one V(4) atom. In the ninth O site, O(9) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(1), and one V(3) atom. In the tenth O site, O(10) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(2), and one V(4) atom. In the eleventh O site, O(11) is bonded in a distorted linear geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(3), and one V(1) atom. In the twelfth O site, O(12) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(4), and one V(2) atom. In the thirteenth O site, O(13) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(1), and one V(3) atom. In the fourteenth O site, O(14) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(2), and one V(4) atom. In the fifteenth O site, O(15) is bonded in a distorted linear geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(3), and one V(1) atom. In the sixteenth O site, O(16) is bonded in a 2-coordinate geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(4), and one V(2) atom. In the seventeenth O site, O(17) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(1), and one V(1) atom. In the eighteenth O site, O(18) is bonded in a 2-coordinate geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(2), and one V(2) atom. In the nineteenth O site, O(19) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(3), and one V(3) atom. In the twentieth O site, O(20) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(4), and one V(4) atom. is represented by the CIF file [CIF]
data_Sr2ZrVO6
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.713
_cell_length_b   11.407
_cell_length_c   8.165
_cell_angle_alpha   89.999
_cell_angle_beta   90.000
_cell_angle_gamma   90.010
_symmetry_Int_Tables_number   1
_cell_volume   532.120
_cell_formula_units_Z   4
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Sr  Sr0  1  0.001  0.251  0.749  1.0
  Sr  Sr1  1  0.500  0.499  0.249  1.0
  Sr  Sr2  1  0.999  0.751  0.750  1.0
  Sr  Sr3  1  0.500  1.000  0.249  1.0
  Sr  Sr4  1  0.001  0.251  0.251  1.0
  Sr  Sr5  1  0.500  0.499  0.751  1.0
  Sr  Sr6  1  0.999  0.750  0.250  1.0
  Sr  Sr7  1  0.500  1.000  0.751  1.0
  Zr  Zr8  1  0.501  0.250  0.000  1.0
  Zr  Zr9  1  0.998  0.500  0.500  1.0
  Zr  Zr10  1  0.499  0.750  1.000  1.0
  Zr  Zr11  1  0.002  0.999  0.500  1.0
  V  V12  1  0.997  0.501  0.000  1.0
  V  V13  1  0.497  0.749  0.500  1.0
  V  V14  1  0.003  0.001  1.000  1.0
  V  V15  1  0.503  0.249  0.500  1.0
  O  O16  1  0.510  0.250  0.744  1.0
  O  O17  1  0.990  0.500  0.244  1.0
  O  O18  1  0.490  0.750  0.744  1.0
  O  O19  1  0.010  1.000  0.244  1.0
  O  O20  1  0.510  0.250  0.256  1.0
  O  O21  1  0.990  0.500  0.756  1.0
  O  O22  1  0.490  0.750  0.256  1.0
  O  O23  1  0.010  1.000  0.756  1.0
  O  O24  1  0.777  0.376  0.000  1.0
  O  O25  1  0.232  0.637  0.500  1.0
  O  O26  1  0.744  0.882  0.000  1.0
  O  O27  1  0.280  0.128  0.500  1.0
  O  O28  1  0.261  0.116  1.000  1.0
  O  O29  1  0.723  0.374  0.500  1.0
  O  O30  1  0.220  0.622  1.000  1.0
  O  O31  1  0.763  0.864  0.500  1.0
  O  O32  1  0.779  0.122  1.000  1.0
  O  O33  1  0.244  0.368  0.500  1.0
  O  O34  1  0.739  0.616  1.000  1.0
  O  O35  1  0.284  0.877  0.500  1.0
  O  O36  1  0.256  0.383  0.000  1.0
  O  O37  1  0.714  0.625  0.500  1.0
  O  O38  1  0.224  0.876  0.000  1.0
  O  O39  1  0.762  0.133  0.500  1.0
[/CIF]
.
The crystal structure described by Sr2ZrVO6 is (Cubic) Perovskite-derived structured and crystallizes in the monoclinic Pm space group. There are four inequivalent Sr sites. In the first Sr site, Sr(1) is bonded to one O(10), one O(13), one O(14), one O(17), one O(2), one O(20), one O(4), one O(5), one O(8), one O(9), and two equivalent O(1) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(1)O12 cuboctahedra, corners with two equivalent Sr(3)O12 cuboctahedra, corners with four equivalent Sr(2)O12 cuboctahedra, corners with four equivalent Sr(4)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(2)O6 octahedra,  a faceface with one Zr(4)O6 octahedra,  a faceface with one V(1)O6 octahedra,  a faceface with one V(3)O6 octahedra, faces with two equivalent Zr(1)O6 octahedra, and faces with two equivalent V(4)O6 octahedra. In the second Sr site, Sr(2) is bonded to one O(1), one O(10), one O(11), one O(14), one O(15), one O(17), one O(18), one O(3), one O(5), one O(6), and two equivalent O(2) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(2)O12 cuboctahedra, corners with two equivalent Sr(4)O12 cuboctahedra, corners with four equivalent Sr(1)O12 cuboctahedra, corners with four equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra,  a faceface with one Zr(1)O6 octahedra,  a faceface with one Zr(3)O6 octahedra,  a faceface with one V(2)O6 octahedra,  a faceface with one V(4)O6 octahedra, faces with two equivalent Zr(2)O6 octahedra, and faces with two equivalent V(1)O6 octahedra. In the third Sr site, Sr(3) is bonded to one O(11), one O(12), one O(15), one O(16), one O(18), one O(19), one O(2), one O(4), one O(6), one O(7), and two equivalent O(3) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(1)O12 cuboctahedra, corners with two equivalent Sr(3)O12 cuboctahedra, corners with four equivalent Sr(2)O12 cuboctahedra, corners with four equivalent Sr(4)O12 cuboctahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(2)O6 octahedra,  a faceface with one Zr(4)O6 octahedra,  a faceface with one V(1)O6 octahedra,  a faceface with one V(3)O6 octahedra, faces with two equivalent Zr(3)O6 octahedra, and faces with two equivalent V(2)O6 octahedra. In the fourth Sr site, Sr(4) is bonded to one O(1), one O(12), one O(13), one O(16), one O(19), one O(20), one O(3), one O(7), one O(8), one O(9), and two equivalent O(4) atoms to form SrO12 cuboctahedra that share corners with two equivalent Sr(2)O12 cuboctahedra, corners with two equivalent Sr(4)O12 cuboctahedra, corners with four equivalent Sr(1)O12 cuboctahedra, corners with four equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra,  a faceface with one Zr(1)O6 octahedra,  a faceface with one Zr(3)O6 octahedra,  a faceface with one V(2)O6 octahedra,  a faceface with one V(4)O6 octahedra, faces with two equivalent Zr(4)O6 octahedra, and faces with two equivalent V(3)O6 octahedra. There are four inequivalent Zr sites. In the first Zr site, Zr(1) is bonded to one O(13), one O(17), one O(5), one O(9), and two equivalent O(1) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(3)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(1)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. In the second Zr site, Zr(2) is bonded to one O(10), one O(14), one O(18), one O(6), and two equivalent O(2) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(2)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-9°. In the third Zr site, Zr(3) is bonded to one O(11), one O(15), one O(19), one O(7), and two equivalent O(3) atoms to form ZrO6 octahedra that share corners with two equivalent V(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(3)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(3)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-6°. In the fourth Zr site, Zr(4) is bonded to one O(12), one O(16), one O(20), one O(8), and two equivalent O(4) atoms to form ZrO6 octahedra that share corners with two equivalent V(2)O6 octahedra, corners with two equivalent V(3)O6 octahedra, corners with two equivalent V(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(4)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-9°. There are four inequivalent V sites. In the first V site, V(1) is bonded to one O(11), one O(15), one O(17), one O(5), and two equivalent O(2) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(2)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-6°. In the second V site, V(2) is bonded to one O(12), one O(16), one O(18), one O(6), and two equivalent O(3) atoms to form VO6 octahedra that share corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(3)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 2-9°. In the third V site, V(3) is bonded to one O(13), one O(19), one O(7), one O(9), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(3)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(1)O12 cuboctahedra, faces with two equivalent Sr(3)O12 cuboctahedra, and faces with four equivalent Sr(4)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. In the fourth V site, V(4) is bonded to one O(10), one O(14), one O(20), one O(8), and two equivalent O(1) atoms to form VO6 octahedra that share corners with two equivalent Zr(1)O6 octahedra, corners with two equivalent Zr(2)O6 octahedra, corners with two equivalent Zr(4)O6 octahedra, faces with two equivalent Sr(2)O12 cuboctahedra, faces with two equivalent Sr(4)O12 cuboctahedra, and faces with four equivalent Sr(1)O12 cuboctahedra. The corner-sharing octahedral tilt angles range from 3-6°. There are twenty inequivalent O sites. In the first O site, O(1) is bonded in a distorted linear geometry to one Sr(2), one Sr(4), two equivalent Sr(1), one Zr(1), and one V(4) atom. In the second O site, O(2) is bonded in a distorted linear geometry to one Sr(1), one Sr(3), two equivalent Sr(2), one Zr(2), and one V(1) atom. In the third O site, O(3) is bonded in a distorted linear geometry to one Sr(2), one Sr(4), two equivalent Sr(3), one Zr(3), and one V(2) atom. In the fourth O site, O(4) is bonded in a distorted linear geometry to one Sr(1), one Sr(3), two equivalent Sr(4), one Zr(4), and one V(3) atom. In the fifth O site, O(5) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(1), and one V(1) atom. In the sixth O site, O(6) is bonded in a 2-coordinate geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(2), and one V(2) atom. In the seventh O site, O(7) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(3), and one V(3) atom. In the eighth O site, O(8) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(4), and one V(4) atom. In the ninth O site, O(9) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(1), and one V(3) atom. In the tenth O site, O(10) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(2), and one V(4) atom. In the eleventh O site, O(11) is bonded in a distorted linear geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(3), and one V(1) atom. In the twelfth O site, O(12) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(4), and one V(2) atom. In the thirteenth O site, O(13) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(1), and one V(3) atom. In the fourteenth O site, O(14) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(2), and one V(4) atom. In the fifteenth O site, O(15) is bonded in a distorted linear geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(3), and one V(1) atom. In the sixteenth O site, O(16) is bonded in a 2-coordinate geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(4), and one V(2) atom. In the seventeenth O site, O(17) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(2), one Zr(1), and one V(1) atom. In the eighteenth O site, O(18) is bonded in a 2-coordinate geometry to two equivalent Sr(2), two equivalent Sr(3), one Zr(2), and one V(2) atom. In the nineteenth O site, O(19) is bonded in a distorted linear geometry to two equivalent Sr(3), two equivalent Sr(4), one Zr(3), and one V(3) atom. In the twentieth O site, O(20) is bonded in a distorted linear geometry to two equivalent Sr(1), two equivalent Sr(4), one Zr(4), and one V(4) atom. is represented by the CIF file [CIF]
data_Sr2ZrVO6
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.713
_cell_length_b   11.407
_cell_length_c   8.165
_cell_angle_alpha   89.999
_cell_angle_beta   90.000
_cell_angle_gamma   90.010
_symmetry_Int_Tables_number   1
_cell_volume   532.120
_cell_formula_units_Z   4
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Sr  Sr0  1  0.001  0.251  0.749  1.0
  Sr  Sr1  1  0.500  0.499  0.249  1.0
  Sr  Sr2  1  0.999  0.751  0.750  1.0
  Sr  Sr3  1  0.500  1.000  0.249  1.0
  Sr  Sr4  1  0.001  0.251  0.251  1.0
  Sr  Sr5  1  0.500  0.499  0.751  1.0
  Sr  Sr6  1  0.999  0.750  0.250  1.0
  Sr  Sr7  1  0.500  1.000  0.751  1.0
  Zr  Zr8  1  0.501  0.250  0.000  1.0
  Zr  Zr9  1  0.998  0.500  0.500  1.0
  Zr  Zr10  1  0.499  0.750  1.000  1.0
  Zr  Zr11  1  0.002  0.999  0.500  1.0
  V  V12  1  0.997  0.501  0.000  1.0
  V  V13  1  0.497  0.749  0.500  1.0
  V  V14  1  0.003  0.001  1.000  1.0
  V  V15  1  0.503  0.249  0.500  1.0
  O  O16  1  0.510  0.250  0.744  1.0
  O  O17  1  0.990  0.500  0.244  1.0
  O  O18  1  0.490  0.750  0.744  1.0
  O  O19  1  0.010  1.000  0.244  1.0
  O  O20  1  0.510  0.250  0.256  1.0
  O  O21  1  0.990  0.500  0.756  1.0
  O  O22  1  0.490  0.750  0.256  1.0
  O  O23  1  0.010  1.000  0.756  1.0
  O  O24  1  0.777  0.376  0.000  1.0
  O  O25  1  0.232  0.637  0.500  1.0
  O  O26  1  0.744  0.882  0.000  1.0
  O  O27  1  0.280  0.128  0.500  1.0
  O  O28  1  0.261  0.116  1.000  1.0
  O  O29  1  0.723  0.374  0.500  1.0
  O  O30  1  0.220  0.622  1.000  1.0
  O  O31  1  0.763  0.864  0.500  1.0
  O  O32  1  0.779  0.122  1.000  1.0
  O  O33  1  0.244  0.368  0.500  1.0
  O  O34  1  0.739  0.616  1.000  1.0
  O  O35  1  0.284  0.877  0.500  1.0
  O  O36  1  0.256  0.383  0.000  1.0
  O  O37  1  0.714  0.625  0.500  1.0
  O  O38  1  0.224  0.876  0.000  1.0
  O  O39  1  0.762  0.133  0.500  1.0
[/CIF]
.